USA Banner
  U.S. flag
              An official website of the United States government Here's how you knowOfficial US Government Icon
              **Official websites use .gov**A **.gov** website belongs to an official government organization in the United States.
            Secure Site Icon
              **Secure .gov websites use HTTPS**
                  A **lock** ( A locked padlock ) or **https://** means you’ve safely connected to the .gov website. Share sensitive information only on official, secure websites. 
 U.S. Department of Transportation Icon United States Department of Transportation
 Search DOT
            Search
                    About FHWAFHWA Organization
                Headquarters Offices
                Field Offices
                Strategic Plan
                Business Opportunities
                Staff Directories
                Careers
                Highway History
                Contact UsProgramsAcquisition Management
                Civil Rights
                Federal Lands Highway
                Infrastructure
                Innovative Program Delivery
                Operations
                Planning, Environment, and Realty
                Policy
                Research, Development, and Technology
                Safety
                Browse by TopicsResourcesCore Highway Topics
                Federal Aid Essentials
                Automation
                Complete Streets
                Laws and Regulations
                Policy & Guidance Center
                Section 508
                Publications and Statistics
                Professional Development
                National Highway Institute
                Resource Center
                Accessibility Resource Library
                FHWA Research LibraryNewsroomPress Releases
                Speeches & Testimony
                Photos
                Videos
                Media ContactsMenu FHWA Highway Safety Programs Home
                        FAQ – HFST – 2017


            
            In This Section
        Pavement Friction
                Friction Management
                Continuous Pavement Friction Measurement (CPFM)
                Traditional Friction Treatments
                High Friction Surface Treatment
                Case Studies and Noteworthy Practices
                FAQs, Links, and Other Resources
                
                LESSONS LEARNED
1. Can patches that de-bond be fixed?

			This is not extremely common, but can be caused by an isolated spot on the pavement that was not cleaned well or had undetected solvent on the pavement. However, if small localized sections of HFST de-bond from the pavement, it can easily be repaired by milling back to a well-bonded area, cleaning the area well, and applying polymer resin and aggregate by hand to blend the patch in with the existing material.
				More common is when a small section "pops out," but the HFST is perfectly attached to a fragment of pavement. If this is a limited occurrence, this does not indicate a catastrophic failure of the HFST. Generally, this means the underlying pavement had a weak spot and lost its bond with a lower layer of pavement. The pavement should be repaired and HFST reapplied if the area is large enough to cause roadway issues. If asphalt is used to patch the pavement, HFST should not be placed for at least 30 days, and if concrete is used, then any curing compound must be removed and the surface cleaned before applying the HFST, since curing compounds act as bond breakers.2. Will the polymer have a reaction with magnesium on a bridge deck?

			No reactions have been found with magnesium chloride deicers. Some concrete repair materials may contain magnesium phosphate and caution is advised. Always consult the HFST resin binder manufacturer prior to the installation of any repair or patching material to confirm compatibility and installation requirements.3. What negative issues have occurred with HFST installation?

			Common contributing issues for installation problems appear to be due to a combination of the following improper practices:
				Improper mixing of the resin binder system, either manually or by automated equipment that did not have fail safes or monitoring devices. This can result in early loss of aggregates and premature wear in the wheelpath. Installations for which the written instructions of the HFST binders have not been followed are always subject to potential problems.
					Improper placement of the resin binder by installing either too thin or too thick a layer of resin material or by disturbing the resin after it has begun its gel phase.
					If the resin material is placed more thinly than indicated by the specification, it may not have sufficient depth to embed and retain the aggregate for long-term durability.
						If the resin material is placed more thickly than indicated by the specification, it may fully encapsulate the aggregate material, leading to a lower friction (glassy) resin surface and lower macrotexture to channel water away. If the material is too thick on steep or banked roadways, it may also exhibit creep or drift towards the lower side of the roadway.
						If the resin is disturbed after placement as it begins to build its strength in the gel phase, it may lead to a reduction in the strength properties of the final cured resin material.
					Application of aggregate after resin binder has begun to gel. Aggregate should be broadcast onto the resin binder immediately to ensure proper embedment. Resin binder tends to gel very fast at high temperatures, and gelled resin binder will resist aggregate embedment. This is a primary advantage of automated continuous application systems which broadcast the aggregate within seconds after placement of the binder resin.
					Improper embedment depth. Embedment depth should typically be 50 percent of the nominal aggregate size to ensure that the aggregate is held firmly in place by the resin binder while still providing adequate texture for frictional resistance and bulk water drainage.
					Application of HFST to immature pavements. The HFST should not be applied to asphalt that is less than 30 days old or concrete pavements less than 28 days old. For concrete pavement, all curing compounds must be removed and the surface properly shot-blasted. Proper shot-blasting will remove all concrete surface paste, dirt, dust, debris and other surface contaminants.
					Application of HFST to pavements in poor condition. Existing pavement may have experienced significant cracking prior to HFST placement, so that over time the asphalt or concrete beneath the HFST failed. In these instances, the resin binder and aggregate have remained completely bonded, but the underlying pavement failed, so it was a poor candidate for HFST.
					Environmental requirements were ignored. The pavement surface must be dry at time of installation, and the ambient temperature must be above the manufacturer’s minimum recommendation. For most polymers, a minimum temperature of 50 degrees F and rising is typical, while some recommend even higher minimum temperatures. Other polymer binders are available that can be installed at lower temperatures per the manufacturers direction. Please see general temperature requirement under INSTALLATION.4. What pavement conditions caused failures that have been reported?

			In North Carolina and in Colorado, two different problems combined to cause the underlying asphalt pavement to be delaminated: poorly draining pavement that trapped water underneath the HFST and cracking of the underlying asphalt pavement that reflected through the HFST. However, the HFST remained intact on the asphalt material.
				Any pattern cracking that is visible on the pavement such as map cracking and/or alligator cracking likely makes the pavement a poor candidate for an HFST installation. Replace un-sound pavement prior to installing HFST to increase service life expectancy. Follow guidelines such as a 28-day hydration period for new concrete pavement and 30 days waiting period for new asphalt pavements prior to installing HFST.
      
  Book traversal links for LESSONS LEARNED
      ‹ MATERIAL SPECIFICATIONS / DURABILITY
                    Up
                    INSTALLATION ›
                
                Book:FAQ – HFST – 2017
              SAFETY
                MAINTENANCE AND OPERATIONS
                COST
                ENVIRONMENTAL IMPACTS
                MATERIAL SPECIFICATIONS / DURABILITY
                LESSONS LEARNED
                INSTALLATION U.S. DEPARTMENT OF TRANSPORTATION

**Federal Highway Administration**

1200 NEW JERSEY AVENUE, SE

WASHINGTON, DC 20590

202-366-4000Subscribe to email updates
                    About
  

        
              About FHWA
                Careers
                Org Chart
                Staff Directories
                Work with UsPrograms
  

        
              Acquisition Management
                Civil Rights
                Federal Lands Highway
                Infrastructure
                Innovative Program Delivery
                Operations
                Planning, Environment, and Realty
                Policy
                Research, Development, and Technology
                SafetyPolicies, Rights, Legal
  

        
              About DOT
                Accessibility
                Budget and Performance
                Civil Rights
                FOIA
                Information Quality
                No FEAR Act
                Office of Inspector General
                Privacy Policy
                USA.gov
                Web Policies and Notices
                Web StandardsNews & Events
  

        
              Newsroom
                Press Releases
                Speeches & Testimony
                Media Contacts
                Connect with Us